#------------------------------------------------------------------------------
#$Date: 2016-02-13 14:50:18 +0200 (Sat, 13 Feb 2016) $
#$Revision: 176428 $
#$URL: svn://www.crystallography.net/cod/cif/1/52/00/1520098.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1520098
loop_
_publ_author_name
'Chen, Lijuan'
'Zhang, Fang'
'Ma, Xing'
'Luo, Jie'
'Zhao, Junwei'
_publ_section_title
;
 Two types of novel tetra-iron substituted sandwich-type arsenotungastates
 with supporting lanthanide pendants.
;
_journal_issue                   28
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              12598
_journal_page_last               12612
_journal_paper_doi               10.1039/c5dt00696a
_journal_volume                  44
_journal_year                    2015
_chemical_formula_sum            'C8 H106 As2 Dy2 Fe4 N2 O116 W18'
_chemical_formula_weight         6094.49
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2015-05-18 deposited with the CCDC.
2015-05-27 downloaded from the CCDC.
;
_cell_angle_alpha                106.8530(10)
_cell_angle_beta                 99.7760(10)
_cell_angle_gamma                97.1530(10)
_cell_formula_units_Z            1
_cell_length_a                   12.6307(11)
_cell_length_b                   13.5293(11)
_cell_length_c                   16.1950(14)
_cell_measurement_reflns_used    8740
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      1.60
_cell_volume                     2565.5(4)
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean none
_diffrn_measured_fraction_theta_full 0.968
_diffrn_measured_fraction_theta_max 0.968
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0328
_diffrn_reflns_av_sigmaI/netI    0.0623
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            12802
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.60
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    22.840
_exptl_absorpt_correction_T_max  0.3411
_exptl_absorpt_correction_T_min  0.0338
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            'Light yellow'
_exptl_crystal_density_diffrn    3.945
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       flaky
_exptl_crystal_F_000             2730
_exptl_crystal_size_max          0.46
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.06
_refine_diff_density_max         2.647
_refine_diff_density_min         -4.784
_refine_diff_density_rms         0.424
_refine_ls_extinction_coef       0.00023(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.042
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     654
_refine_ls_number_reflns         8740
_refine_ls_number_restraints     37
_refine_ls_restrained_S_all      1.040
_refine_ls_R_factor_all          0.0543
_refine_ls_R_factor_gt           0.0489
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0639P)²+63.4873P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1233
_refine_ls_wR_factor_ref         0.1265
_reflns_number_gt                7837
_reflns_number_total             8740
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5dt00696a3.cif
_cod_data_source_block           12-Dy
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 3271 2015-04-21 07:52:19Z andrius 

 Adding full bibliography for 1520091--1520099.cif.
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               1520098
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.21089(5) 0.31191(4) 0.59396(4) 0.01475(15) Uani 1 1 d . . .
W2 W 0.46649(4) 0.44245(4) 0.67933(4) 0.01367(15) Uani 1 1 d . . .
W3 W 0.24561(5) 0.57536(4) 0.75400(4) 0.01349(15) Uani 1 1 d . . .
W4 W 0.35717(4) 0.61342(4) 0.97108(4) 0.00994(15) Uani 1 1 d . . .
W5 W 0.09441(4) 0.48649(4) 0.87831(4) 0.01245(15) Uani 1 1 d . . .
W6 W 0.15058(5) 0.25681(4) 0.94473(4) 0.01438(15) Uani 1 1 d . . .
W7 W 0.24593(5) 0.08956(4) 0.79027(4) 0.01461(16) Uani 1 1 d . . .
W8 W 0.41218(5) 0.18425(4) 0.65272(4) 0.01580(16) Uani 1 1 d . . .
W9 W 0.04202(4) 0.21332(4) 0.73107(4) 0.01364(15) Uani 1 1 d . . .
Dy1 Dy 0.11779(8) 0.24097(8) 0.33104(7) 0.0415(2) Uani 1 1 d . . .
As1 As 0.33889(11) 0.35944(10) 0.83518(9) 0.0084(3) Uani 1 1 d . . .
Fe1 Fe 0.38174(15) 0.42986(15) 1.10037(14) 0.0120(4) Uani 1 1 d . . .
O1W O 0.2410(8) 0.4510(9) 1.1551(8) 0.027(3) Uani 1 1 d . . .
O2W O 0.4082(10) 0.3159(9) 1.1644(8) 0.030(3) Uani 1 1 d . . .
O3W O 0.5532(12) 0.0495(9) 0.9311(9) 0.040(3) Uani 1 1 d . . .
O4W O 0.6867(9) 0.1198(10) 0.8229(10) 0.039(3) Uani 1 1 d . . .
O5W O 0.247(2) 0.1466(16) 0.3791(17) 0.105(9) Uani 1 1 d . . .
O6W O 0.2746(15) 0.3764(14) 0.4049(12) 0.069(5) Uani 1 1 d . . .
O7W O -0.048(3) 0.177(2) 0.219(2) 0.069(8) Uiso 0.60 1 d P . .
O7M O -0.050(3) 0.215(3) 0.344(3) 0.062(11) Uiso 0.40 1 d P . .
O8W O 0.067(3) 0.068(3) 0.227(3) 0.167(13) Uiso 1 1 d . . .
O9W O 0.2376(19) 0.224(2) 0.2296(15) 0.110(9) Uani 1 1 d . . .
O10W O 0.090(4) 0.343(4) 0.236(3) 0.121(14) Uiso 0.65 1 d P . .
O10M O 0.035(4) 0.296(4) 0.201(4) 0.062(13) Uiso 0.35 1 d P . .
O11W O 0.019(3) 0.102(3) 0.372(3) 0.095(11) Uiso 0.60 1 d P . .
O11M O -0.072(9) 0.012(8) 0.388(7) 0.18(4) Uiso 0.40 1 d P . .
O12W O 0.060(3) 0.407(3) 0.376(2) 0.073(9) Uiso 0.60 1 d P . .
O12M O -0.011(4) 0.340(4) 0.381(4) 0.078(14) Uiso 0.40 1 d P . .
O13W O -0.117(2) 0.196(2) 0.064(2) 0.127(9) Uiso 1 1 d . . .
O14W O 0.766(4) -0.011(4) 0.911(3) 0.098(14) Uiso 0.50 1 d P . .
O15W O 0.146(15) 0.556(14) 0.503(14) 0.39(10) Uiso 0.50 1 d P . .
O16W O 0.310(3) -0.051(3) 0.360(2) 0.083(10) Uiso 0.60 1 d P . .
O16M O 0.319(4) -0.135(4) 0.416(4) 0.084(15) Uiso 0.40 1 d P . .
O17W O 0.3793(17) 0.1337(12) 1.0406(11) 0.070(5) Uani 1 1 d . . .
O18W O 0.368(2) -0.1209(19) 0.8939(17) 0.059(6) Uiso 0.70 1 d P . .
O18M O 0.303(4) -0.128(4) 0.913(3) 0.045(11) Uiso 0.30 1 d P . .
O19W O -0.1650(11) 0.2894(11) 0.8701(10) 0.043(3) Uani 1 1 d . . .
O20W O 0.7401(14) 0.3507(14) 0.7263(14) 0.079(6) Uani 1 1 d . . .
O21W O -0.0985(17) 0.3971(15) 0.6319(13) 0.080(6) Uani 1 1 d . . .
O22W O 0.1162(18) 0.0012(17) 0.5080(16) 0.088(6) Uiso 1 1 d . . .
O23W O 0.1342(16) -0.2037(16) 0.5114(12) 0.073(5) Uani 1 1 d . . .
O1 O 0.1320(9) 0.2919(8) 0.4892(7) 0.024(3) Uani 1 1 d . . .
O2 O 0.2856(8) 0.1971(8) 0.5670(7) 0.018(2) Uani 1 1 d . . .
O3 O 0.1812(8) 0.4401(7) 0.6638(7) 0.017(2) Uani 1 1 d . . .
O4 O 0.3380(8) 0.3315(7) 0.7191(6) 0.013(2) Uani 1 1 d . . .
O5 O 0.1128(8) 0.2388(7) 0.6415(7) 0.016(2) Uani 1 1 d . . .
O6 O 0.3379(8) 0.3952(8) 0.5817(7) 0.020(2) Uani 1 1 d . . .
O7 O 0.5545(9) 0.5126(9) 0.6371(8) 0.027(3) Uani 1 1 d . . .
O8 O 0.4942(8) 0.3017(7) 0.6334(7) 0.017(2) Uani 1 1 d . . .
O9 O 0.5435(8) 0.4619(7) 0.7892(7) 0.018(2) Uani 1 1 d . . .
O10 O 0.3828(8) 0.5489(7) 0.7281(7) 0.017(2) Uani 1 1 d . . .
O11 O 0.2211(9) 0.6656(9) 0.6998(8) 0.025(2) Uani 1 1 d . . .
O12 O 0.1105(8) 0.5591(7) 0.7924(7) 0.015(2) Uani 1 1 d . . .
O13 O 0.2720(7) 0.4715(7) 0.8499(7) 0.016(2) Uani 1 1 d . . .
O14 O 0.3143(8) 0.6671(7) 0.8672(7) 0.013(2) Uani 1 1 d U . .
O15 O 0.4818(8) 0.5916(8) 0.9386(7) 0.019(2) Uani 1 1 d . . .
O16 O 0.3557(8) 0.5273(7) 1.0359(7) 0.016(2) Uani 1 1 d . . .
O17 O 0.3938(8) 0.7404(7) 1.0510(7) 0.016(2) Uani 1 1 d . . .
O18 O 0.1925(7) 0.6004(7) 0.9641(6) 0.012(2) Uani 1 1 d U . .
O19 O -0.0288(8) 0.5183(8) 0.8986(8) 0.025(3) Uani 1 1 d . . .
O20 O 0.0458(8) 0.3606(8) 0.7759(7) 0.017(2) Uani 1 1 d . . .
O21 O 0.1217(8) 0.3942(7) 0.9439(7) 0.015(2) Uani 1 1 d . . .
O22 O 0.2213(8) 0.2613(7) 0.8211(7) 0.013(2) Uani 1 1 d . . .
O23 O 0.2897(8) 0.3131(7) 1.0055(6) 0.014(2) Uani 1 1 d U . .
O24 O 0.0853(9) 0.2364(8) 1.0250(7) 0.022(2) Uani 1 1 d U . .
O25 O 0.0206(9) 0.2104(8) 0.8431(9) 0.027(3) Uani 1 1 d . . .
O26 O 0.1803(8) 0.1184(8) 0.8929(7) 0.019(2) Uani 1 1 d . . .
O27 O 0.2312(9) -0.0459(7) 0.7666(8) 0.023(2) Uani 1 1 d . . .
O28 O 0.0986(8) 0.0870(8) 0.7193(7) 0.018(2) Uani 1 1 d . . .
O29 O 0.3813(9) 0.1382(8) 0.8600(7) 0.019(2) Uani 1 1 d . . .
O30 O 0.3010(8) 0.1084(8) 0.6931(7) 0.018(2) Uani 1 1 d . . .
O31 O 0.4521(10) 0.0798(10) 0.5816(8) 0.033(3) Uani 1 1 d . . .
O32 O 0.5065(8) 0.2058(8) 0.7595(8) 0.023(2) Uani 1 1 d . . .
O33 O -0.0897(8) 0.1673(8) 0.6710(8) 0.023(2) Uani 1 1 d . . .
O34 O 0.4817(10) -0.0062(8) 0.7482(8) 0.028(3) Uani 1 1 d D . .
Fe2 Fe 0.53287(16) 0.13553(15) 0.84566(14) 0.0151(4) Uani 1 1 d . . .
O35 O 0.619(2) -0.043(2) 0.680(2) 0.055(6) Uiso 0.50 1 d PD . 1
O36 O 0.510(4) -0.270(4) 0.662(3) 0.090(9) Uiso 0.50 1 d PD A 1
H36 H 0.5334 -0.3258 0.6491 0.135 Uiso 0.50 1 d PR A 1
N1 N 0.332(2) -0.144(3) 0.627(3) 0.043(6) Uiso 0.50 1 d PD A 1
H1A H 0.2954 -0.1958 0.5792 0.051 Uiso 0.50 1 d PR A 1
H1B H 0.3237 -0.1594 0.6746 0.051 Uiso 0.50 1 d PR A 1
H1C H 0.3063 -0.0851 0.6276 0.051 Uiso 0.50 1 d PR A 1
C1 C 0.521(2) -0.057(3) 0.687(2) 0.032(6) Uiso 0.50 1 d PD A 1
C2 C 0.449(3) -0.144(2) 0.609(3) 0.046(7) Uiso 0.50 1 d PD A 1
H2 H 0.4526 -0.1273 0.5545 0.055 Uiso 0.50 1 calc PR A 1
C3 C 0.461(3) -0.2574(19) 0.5953(19) 0.072(8) Uani 1 1 d DU . .
C4 C 0.384(2) -0.347(2) 0.533(2) 0.073(7) Uani 1 1 d U A .
H4A H 0.3557 -0.3305 0.4815 0.110 Uiso 1 1 d R . .
H4B H 0.4202 -0.4059 0.5177 0.110 Uiso 1 1 d R . .
H4C H 0.3259 -0.3627 0.5603 0.110 Uiso 1 1 d R . .
O35' O 0.581(2) -0.121(2) 0.763(2) 0.055(6) Uiso 0.50 1 d PD A 2
O36' O 0.523(4) -0.219(4) 0.557(3) 0.090(9) Uiso 0.50 1 d PD A 2
H36' H 0.5079 -0.1630 0.5524 0.135 Uiso 0.50 1 d PR A 2
N1' N 0.343(3) -0.116(3) 0.600(2) 0.043(6) Uiso 0.50 1 d PD A 2
H1'A H 0.2927 -0.1590 0.5543 0.064 Uiso 0.50 1 d PR A 2
H1'B H 0.3115 -0.0685 0.6331 0.064 Uiso 0.50 1 d PR A 2
H1'C H 0.3930 -0.0829 0.5798 0.064 Uiso 0.50 1 d PR A 2
C1' C 0.490(3) -0.099(2) 0.734(2) 0.032(6) Uiso 0.50 1 d PD A 2
C2' C 0.411(3) -0.174(3) 0.652(2) 0.046(7) Uiso 0.50 1 d PD A 2
H2' H 0.3581 -0.2129 0.6747 0.055 Uiso 0.50 1 calc PR A 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Dy Dy -0.1892 4.4098 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 W1 O5 100.9(5) . .
O1 W1 O3 103.8(4) . .
O5 W1 O3 88.9(4) . .
O1 W1 O2 99.4(4) . .
O5 W1 O2 91.4(4) . .
O3 W1 O2 156.3(4) . .
O1 W1 O6 97.0(5) . .
O5 W1 O6 162.1(5) . .
O3 W1 O6 86.2(4) . .
O2 W1 O6 86.3(4) . .
O1 W1 O4 170.2(4) . .
O5 W1 O4 86.2(4) . .
O3 W1 O4 83.0(4) . .
O2 W1 O4 73.4(4) . .
O6 W1 O4 76.2(4) . .
O7 W2 O9 102.9(5) . .
O7 W2 O8 101.7(5) . .
O9 W2 O8 93.4(4) . .
O7 W2 O10 100.7(5) . .
O9 W2 O10 89.9(4) . .
O8 W2 O10 155.9(4) . .
O7 W2 O6 100.8(5) . .
O9 W2 O6 156.1(5) . .
O8 W2 O6 84.8(4) . .
O10 W2 O6 82.6(4) . .
O7 W2 O4 172.9(5) . .
O9 W2 O4 83.1(4) . .
O8 W2 O4 73.8(4) . .
O10 W2 O4 83.0(4) . .
O6 W2 O4 73.5(4) . .
O11 W3 O14 99.8(5) . .
O11 W3 O10 100.4(5) . .
O14 W3 O10 91.2(4) . .
O11 W3 O12 99.2(5) . .
O14 W3 O12 89.9(4) . .
O10 W3 O12 159.9(4) . .
O11 W3 O3 103.6(5) . .
O14 W3 O3 156.5(4) . .
O10 W3 O3 86.7(4) . .
O12 W3 O3 84.3(4) . .
O11 W3 O13 170.2(5) . .
O14 W3 O13 72.5(4) . .
O10 W3 O13 86.1(4) . .
O12 W3 O13 75.1(4) . .
O3 W3 O13 84.0(4) . .
O17 W4 O15 103.0(5) . .
O17 W4 O16 103.6(5) . .
O15 W4 O16 96.9(5) . .
O17 W4 O14 94.6(4) . .
O15 W4 O14 89.6(4) . .
O16 W4 O14 158.6(4) . .
O17 W4 O18 95.8(4) . .
O15 W4 O18 159.3(4) . .
O16 W4 O18 86.7(4) . .
O14 W4 O18 80.3(4) . .
O17 W4 O13 163.4(4) . .
O15 W4 O13 87.1(4) . .
O16 W4 O13 88.0(4) . .
O14 W4 O13 72.0(4) . .
O18 W4 O13 72.7(3) . .
O19 W5 O18 100.6(5) . .
O19 W5 O21 103.1(5) . .
O18 W5 O21 92.8(4) . .
O19 W5 O20 101.2(5) . .
O18 W5 O20 157.8(4) . .
O21 W5 O20 85.9(4) . .
O19 W5 O12 98.1(5) . .
O18 W5 O12 88.2(4) . .
O21 W5 O12 158.3(4) . .
O20 W5 O12 85.0(4) . .
O19 W5 O13 170.6(4) . .
O18 W5 O13 73.4(4) . .
O21 W5 O13 84.7(4) . .
O20 W5 O13 84.4(4) . .
O12 W5 O13 74.7(4) . .
O24 W6 O23 102.9(5) . .
O24 W6 O26 100.9(5) . .
O23 W6 O26 95.1(4) . .
O24 W6 O21 101.6(5) . .
O23 W6 O21 91.2(4) . .
O26 W6 O21 154.6(4) . .
O24 W6 O25 98.3(5) . .
O23 W6 O25 158.5(5) . .
O26 W6 O25 83.8(4) . .
O21 W6 O25 81.4(4) . .
O24 W6 O22 171.3(4) . .
O23 W6 O22 84.3(4) . .
O26 W6 O22 73.4(4) . .
O21 W6 O22 82.8(4) . .
O25 W6 O22 74.8(4) . .
O27 W7 O29 103.5(5) . .
O27 W7 O30 101.2(5) . .
O29 W7 O30 89.8(5) . .
O27 W7 O26 97.8(5) . .
O29 W7 O26 91.1(5) . .
O30 W7 O26 160.2(4) . .
O27 W7 O28 95.7(5) . .
O29 W7 O28 160.8(4) . .
O30 W7 O28 85.8(4) . .
O26 W7 O28 86.8(4) . .
O27 W7 O22 166.2(4) . .
O29 W7 O22 87.9(4) . .
O30 W7 O22 86.3(4) . .
O26 W7 O22 74.0(4) . .
O28 W7 O22 73.1(4) . .
O31 W8 O32 103.0(5) . .
O31 W8 O8 101.2(5) . .
O32 W8 O8 92.1(5) . .
O31 W8 O30 100.2(5) . .
O32 W8 O30 88.4(5) . .
O8 W8 O30 157.9(4) . .
O31 W8 O2 97.5(5) . .
O32 W8 O2 159.2(4) . .
O8 W8 O2 87.6(4) . .
O30 W8 O2 84.3(4) . .
O31 W8 O4 166.9(5) . .
O32 W8 O4 89.6(4) . .
O8 W8 O4 74.2(4) . .
O30 W8 O4 83.7(4) . .
O2 W8 O4 70.3(4) . .
O33 W9 O25 99.5(5) . .
O33 W9 O20 102.4(5) . .
O25 W9 O20 85.7(5) . .
O33 W9 O28 102.2(5) . .
O25 W9 O28 87.7(5) . .
O20 W9 O28 155.2(4) . .
O33 W9 O5 100.1(5) . .
O25 W9 O5 160.3(4) . .
O20 W9 O5 88.1(4) . .
O28 W9 O5 90.1(4) . .
O33 W9 O22 173.5(4) . .
O25 W9 O22 76.0(4) . .
O20 W9 O22 82.1(4) . .
O28 W9 O22 73.2(4) . .
O5 W9 O22 84.6(4) . .
O7M Dy1 O12M 41.6(17) . .
O7M Dy1 O5W 122.6(14) . .
O12M Dy1 O5W 140.9(15) . .
O7M Dy1 O10W 95.4(17) . .
O12M Dy1 O10W 75.1(18) . .
O5W Dy1 O10W 140.3(14) . .
O7M Dy1 O8W 83.5(15) . .
O12M Dy1 O8W 122.5(16) . .
O5W Dy1 O8W 75.0(11) . .
O10W Dy1 O8W 100.7(16) . .
O7M Dy1 O6W 134.9(13) . .
O12M Dy1 O6W 96.0(14) . .
O5W Dy1 O6W 77.8(7) . .
O10W Dy1 O6W 83.3(13) . .
O8W Dy1 O6W 141.2(11) . .
O7M Dy1 O12W 70.6(14) . .
O12M Dy1 O12W 29.6(14) . .
O5W Dy1 O12W 141.2(10) . .
O10W Dy1 O12W 57.9(14) . .
O8W Dy1 O12W 143.2(12) . .
O6W Dy1 O12W 70.9(9) . .
O7M Dy1 O9W 145.2(13) . .
O12M Dy1 O9W 141.1(16) . .
O5W Dy1 O9W 75.0(11) . .
O10W Dy1 O9W 66.4(14) . .
O8W Dy1 O9W 72.0(12) . .
O6W Dy1 O9W 74.6(8) . .
O12W Dy1 O9W 116.3(11) . .
O7M Dy1 O7W 49.8(14) . .
O12M Dy1 O7W 72.9(15) . .
O5W Dy1 O7W 129.2(9) . .
O10W Dy1 O7W 65.6(15) . .
O8W Dy1 O7W 54.9(12) . .
O6W Dy1 O7W 148.6(9) . .
O12W Dy1 O7W 88.2(11) . .
O9W Dy1 O7W 95.5(10) . .
O7M Dy1 O1 76.5(12) . .
O12M Dy1 O1 65.6(13) . .
O5W Dy1 O1 76.2(7) . .
O10W Dy1 O1 128.8(12) . .
O8W Dy1 O1 127.6(10) . .
O6W Dy1 O1 70.1(5) . .
O12W Dy1 O1 72.0(9) . .
O9W Dy1 O1 138.2(6) . .
O7W Dy1 O1 126.3(8) . .
O7M Dy1 O11W 50.6(15) . .
O12M Dy1 O11W 86.0(16) . .
O5W Dy1 O11W 72.6(12) . .
O10W Dy1 O11W 140.5(16) . .
O8W Dy1 O11W 61.1(14) . .
O6W Dy1 O11W 133.8(10) . .
O12W Dy1 O11W 114.5(12) . .
O9W Dy1 O11W 128.0(12) . .
O7W Dy1 O11W 75.8(12) . .
O1 Dy1 O11W 68.9(10) . .
O7M Dy1 O10M 82.6(17) . .
O12M Dy1 O10M 74.9(18) . .
O5W Dy1 O10M 144.1(14) . .
O10W Dy1 O10M 19.9(13) . .
O8W Dy1 O10M 84.1(16) . .
O6W Dy1 O10M 103.1(14) . .
O12W Dy1 O10M 67.3(14) . .
O9W Dy1 O10M 70.9(14) . .
O7W Dy1 O10M 46.0(15) . .
O1 Dy1 O10M 138.5(12) . .
O11W Dy1 O10M 121.7(16) . .
O22 As1 O13 98.0(4) . .
O22 As1 O4 96.1(4) . .
O13 As1 O4 98.3(5) . .
O16 Fe1 O23 92.3(4) . .
O16 Fe1 O9 94.8(4) . 2_667
O23 Fe1 O9 168.4(5) . 2_667
O16 Fe1 O15 92.5(4) . 2_667
O23 Fe1 O15 95.6(4) . 2_667
O9 Fe1 O15 93.2(4) 2_667 2_667
O16 Fe1 O2W 176.8(5) . .
O23 Fe1 O2W 84.7(4) . .
O9 Fe1 O2W 88.3(4) 2_667 .
O15 Fe1 O2W 86.5(5) 2_667 .
O16 Fe1 O1W 92.5(5) . .
O23 Fe1 O1W 87.4(4) . .
O9 Fe1 O1W 83.2(5) 2_667 .
O15 Fe1 O1W 174.1(5) 2_667 .
O2W Fe1 O1W 88.7(5) . .
O12M O7M Dy1 75(2) . .
O10M O10W Dy1 91(5) . .
O10W O10M Dy1 69(5) . .
O11M O11W Dy1 168(4) . .
O11W O11M O28 99(6) . 2_556
O12M O12W Dy1 72(3) . .
O12W O12M O7M 139(5) . .
O12W O12M Dy1 78(3) . .
O7M O12M Dy1 63(2) . .
O16M O16W O35 147(3) . 2_656
W1 O1 Dy1 148.4(6) . .
W1 O2 W8 121.9(5) . .
W1 O3 W3 144.9(6) . .
As1 O4 W1 136.0(5) . .
As1 O4 W8 116.5(4) . .
W1 O4 W8 94.1(3) . .
As1 O4 W2 117.4(4) . .
W1 O4 W2 91.3(3) . .
W8 O4 W2 90.6(3) . .
W1 O5 W9 156.4(6) . .
W1 O6 W2 118.7(5) . .
W8 O8 W2 121.4(5) . .
W2 O9 Fe1 142.9(6) . 2_667
W3 O10 W2 146.1(5) . .
W3 O12 W5 120.6(5) . .
As1 O13 W4 114.4(5) . .
As1 O13 W5 128.9(5) . .
W4 O13 W5 93.3(3) . .
As1 O13 W3 127.6(5) . .
W4 O13 W3 93.7(3) . .
W5 O13 W3 89.4(3) . .
W3 O14 W4 121.7(5) . .
W4 O15 Fe1 178.0(7) . 2_667
W4 O16 Fe1 168.6(6) . .
W4 O17 Fe2 164.1(6) . 2_667
W5 O18 W4 120.3(5) . .
W9 O20 W5 145.6(6) . .
W5 O21 W6 148.1(6) . .
As1 O22 W7 117.2(4) . .
As1 O22 W6 118.8(5) . .
W7 O22 W6 92.5(3) . .
As1 O22 W9 134.7(5) . .
W7 O22 W9 93.0(3) . .
W6 O22 W9 90.5(3) . .
W6 O23 Fe1 144.7(6) . .
W9 O25 W6 118.4(5) . .
W6 O26 W7 120.0(5) . .
O11M O28 W9 120(4) 2_556 .
O11M O28 W7 111(3) 2_556 .
W9 O28 W7 120.5(5) . .
W7 O29 Fe2 136.8(6) . .
W7 O30 W8 147.2(6) . .
W8 O32 Fe2 138.4(6) . .
C1' O34 C1 56(2) . .
C1' O34 Fe2 140.2(18) . .
C1 O34 Fe2 134.5(17) . .
O32 Fe2 O29 88.7(5) . .
O32 Fe2 O17 98.4(5) . 2_667
O29 Fe2 O17 98.1(4) . 2_667
O32 Fe2 O34 89.9(5) . .
O29 Fe2 O34 89.9(4) . .
O17 Fe2 O34 168.5(5) 2_667 .
O32 Fe2 O3W 175.4(5) . .
O29 Fe2 O3W 89.8(5) . .
O17 Fe2 O3W 86.0(5) 2_667 .
O34 Fe2 O3W 85.8(5) . .
O32 Fe2 O4W 91.7(5) . .
O29 Fe2 O4W 175.0(5) . .
O17 Fe2 O4W 86.8(5) 2_667 .
O34 Fe2 O4W 85.1(5) . .
O3W Fe2 O4W 89.4(6) . .
C1 O35 O16W 129(3) . 2_656
O34 C1 O35 127(3) . .
O34 C1 C2 121(3) . .
O35 C1 C2 112(3) . .
C3 C2 C1 120(3) . .
C3 C2 N1 103(3) . .
C1 C2 N1 104(3) . .
O36 C3 O36' 112(4) . .
O36 C3 C4 117(3) . .
O36' C3 C4 110(3) . .
O36 C3 C2 113(3) . .
O36' C3 C2 71(3) . .
C4 C3 C2 124(3) . .
O36 C3 C2' 90(3) . .
O36' C3 C2' 111(3) . .
C4 C3 C2' 116(3) . .
C2 C3 C2' 41(2) . .
O34 C1' O35' 119(3) . .
O34 C1' C2' 115(3) . .
O35' C1' C2' 121(3) . .
C3 C2' C1' 115(3) . .
C3 C2' N1' 114(3) . .
C1' C2' N1' 112(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O1 1.743(11) .
W1 O5 1.889(10) .
W1 O3 1.897(10) .
W1 O2 1.900(10) .
W1 O6 1.916(10) .
W1 O4 2.288(10) .
W2 O7 1.725(11) .
W2 O9 1.805(10) .
W2 O8 1.932(9) .
W2 O10 1.954(10) .
W2 O6 1.957(11) .
W2 O4 2.369(10) .
W3 O11 1.726(11) .
W3 O14 1.878(10) .
W3 O10 1.903(10) .
W3 O12 1.921(10) .
W3 O3 1.954(10) .
W3 O13 2.389(10) .
W4 O17 1.775(9) .
W4 O15 1.775(10) .
W4 O16 1.780(10) .
W4 O14 2.037(10) .
W4 O18 2.046(9) .
W4 O13 2.298(10) .
W5 O19 1.724(10) .
W5 O18 1.881(9) .
W5 O21 1.886(10) .
W5 O20 1.945(10) .
W5 O12 1.946(10) .
W5 O13 2.386(9) .
W6 O24 1.721(11) .
W6 O23 1.811(10) .
W6 O26 1.929(10) .
W6 O21 1.942(10) .
W6 O25 2.006(12) .
W6 O22 2.339(10) .
W7 O27 1.739(10) .
W7 O29 1.807(10) .
W7 O30 1.894(11) .
W7 O26 1.943(11) .
W7 O28 2.005(10) .
W7 O22 2.303(9) .
W8 O31 1.734(12) .
W8 O32 1.848(11) .
W8 O8 1.920(10) .
W8 O30 1.948(10) .
W8 O2 1.992(11) .
W8 O4 2.360(9) .
W9 O33 1.716(10) .
W9 O25 1.890(13) .
W9 O20 1.905(10) .
W9 O28 1.905(10) .
W9 O5 1.917(11) .
W9 O22 2.374(10) .
Dy1 O7M 2.16(4) .
Dy1 O12M 2.34(5) .
Dy1 O5W 2.35(2) .
Dy1 O10W 2.36(5) .
Dy1 O8W 2.38(4) .
Dy1 O6W 2.394(15) .
Dy1 O12W 2.40(3) .
Dy1 O9W 2.40(2) .
Dy1 O7W 2.40(3) .
Dy1 O1 2.421(12) .
Dy1 O11W 2.44(4) .
Dy1 O10M 2.53(5) .
As1 O22 1.800(9) .
As1 O13 1.802(9) .
As1 O4 1.804(10) .
Fe1 O16 1.931(10) .
Fe1 O23 1.933(10) .
Fe1 O9 1.949(10) 2_667
Fe1 O15 1.959(10) 2_667
Fe1 O2W 2.121(12) .
Fe1 O1W 2.132(11) .
O3W Fe2 2.055(13) .
O4W Fe2 2.064(12) .
O7M O12M 1.61(7) .
O10W O10M 0.86(6) .
O11W O11M 1.67(11) .
O11M O28 1.81(11) 2_556
O12W O12M 1.21(6) .
O16W O16M 1.65(7) .
O16W O35 1.79(5) 2_656
O18W O18M 0.93(5) .
O9 Fe1 1.949(10) 2_667
O15 Fe1 1.959(10) 2_667
O17 Fe2 1.984(10) 2_667
O28 O11M 1.81(11) 2_556
O29 Fe2 1.971(11) .
O32 Fe2 1.911(11) .
O34 C1' 1.23(3) .
O34 C1 1.24(3) .
O34 Fe2 2.043(11) .
Fe2 O17 1.984(10) 2_667
O35 C1 1.27(3) .
O35 O16W 1.79(5) 2_656
O36 C3 1.22(4) .
N1 C2 1.56(4) .
C1 C2 1.52(4) .
C2 C3 1.51(4) .
C3 O36' 1.23(4) .
C3 C4 1.44(4) .
C3 C2' 1.51(4) .
O35' C1' 1.27(3) .
N1' C2' 1.55(4) .
C1' C2' 1.52(4) .
